#------------------------------------------------------------------------------
#$Date: 2016-02-13 21:28:24 +0200 (Sat, 13 Feb 2016) $
#$Revision: 176429 $
#$URL: svn://www.crystallography.net/cod/cif/4/00/26/4002613.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4002613
loop_
_publ_author_name
'Ishizawa, Nobuo'
'Asaka, Toru'
'Kudo, Tatsunari'
'Fukuda, Koichiro'
'Yasuhara, Akira'
'Abe, Nobuyuki'
'Arima, Taka-hisa'
_publ_section_title
;
 Structural Evolution of GdBaCo2O5+δ(δ = 7/18) at Elevated Temperatures
;
_journal_name_full               'Chemistry of Materials'
_journal_page_first              141114094038007
_journal_paper_doi               10.1021/cm503132e
_journal_year                    2014
_chemical_formula_sum            'Ba Co2 Gd O5.19'
_chemical_formula_weight         495.5
_chemical_name_systematic        ' ?'
_space_group_IT_number           123
_symmetry_cell_setting           tetragonal
_symmetry_Int_Tables_number      123
_symmetry_space_group_name_Hall  '-P 4 2'
_symmetry_space_group_name_H-M   'P 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.8984(4)
_cell_length_b                   3.8984(4)
_cell_length_c                   7.5532(16)
_cell_measurement_temperature    404
_cell_volume                     114.79(3)
_diffrn_ambient_temperature      404
_diffrn_measured_fraction_theta_full 0.96
_diffrn_measured_fraction_theta_max 0.96
_diffrn_measurement_device       'four-cycle diffractometer'
_diffrn_measurement_device_type  'Bruker CCD'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0193
_diffrn_reflns_av_sigmaI/netI    0.0146
_diffrn_reflns_limit_h_max       5
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       4
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -3
_diffrn_reflns_number            620
_diffrn_reflns_theta_full        30.1
_diffrn_reflns_theta_max         30.1
_diffrn_reflns_theta_min         5.89
_exptl_absorpt_coefficient_mu    29.74
_exptl_absorpt_correction_T_max  0.1240
_exptl_absorpt_correction_T_min  0.0681
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   '(SADABS; Sheldrick, 1996)'
_exptl_crystal_density_diffrn    7.1677
_exptl_crystal_description       'triangular pyramidal'
_exptl_crystal_F_000             216
_exptl_crystal_size_max          0.1
_exptl_crystal_size_mid          0.1
_exptl_crystal_size_min          0.075
_refine_diff_density_max         1.16
_refine_diff_density_min         -0.89
_refine_ls_extinction_coef       300(20)
_refine_ls_extinction_method
'B-C type 1 Gaussian isotropic (Becker & Coppens, 1974)'
_refine_ls_goodness_of_fit_gt    1.92
_refine_ls_goodness_of_fit_ref   1.82
_refine_ls_number_constraints    0
_refine_ls_number_parameters     16
_refine_ls_number_reflns         132
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0240
_refine_ls_R_factor_gt           0.0229
_refine_ls_shift/su_max          0.0061
_refine_ls_shift/su_mean         0.0012
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     w=1/(σ²(F)+0.0001F²)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0267
_refine_ls_wR_factor_ref         0.0272
_reflns_number_gt                117
_reflns_number_total             132
_reflns_threshold_expression     I>3σ(I)
_cod_data_source_file            cm503132e_si_002.cif
_cod_data_source_block           c130
_cod_depositor_comments
;
The following automatic conversions were performed:

'_diffrn_radiation_probe' value 'X-ray' changed to 'x-ray' according
to /home/saulius/struct/CIF-dictionaries/IUCr/cif_core.dic dictionary
named 'cif_core.dic' version 2.4.5 from 2014-11-21.

Automatic conversion script
Id: cif_fix_values 3866 2015-08-17 15:13:47Z robertas 
;
_cod_original_sg_symbol_Hall     '-P 4;-2'
_cod_original_formula_sum        'Ba1 Co2 Gd1 O5.19'
_cod_database_code               4002613
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -x,-y,z
3 -y,x,z
4 y,-x,z
5 -x,y,-z
6 x,-y,-z
7 y,x,-z
8 -y,-x,-z
9 -x,-y,-z
10 x,y,-z
11 y,-x,-z
12 -y,x,-z
13 x,-y,z
14 -x,y,z
15 -y,-x,z
16 y,x,z
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_adp_type
_atom_site_U_iso_or_equiv
_atom_site_site_symmetry_multiplicity
_atom_site_occupancy
_atom_site_calc_flag
Gd1 Gd 0 0 0.5 Uani 0.0257(2) 1 1 d
Ba1 Ba 0 0 0 Uani 0.0208(2) 1 1 d
Co1 Co 0.5 0.5 0.25460(10) Uani 0.0195(3) 2 1 d
O1 O 0.5 0.5 0 Uani 0.0242(16) 1 1 d
O2 O 0.5 0 0.3025(6) Uani 0.0280(11) 4 1 d
O3 O 0.5 0.5 0.5 Uiso 0.033(10) 1 0.19 d
loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ba -0.3244 2.2819 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Co 0.3494 0.9721 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Gd -0.1653 3.9035 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
O 0.0106 0.0060 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
O2 Gd1 O2 1_455 . 105.14(13)
O2 Gd1 O2 1_455 3_545 68.32(7)
O2 Gd1 O2 1_455 3_555 68.32(7)
O2 Gd1 O2 1_455 5_556 74.86(13)
O2 Gd1 O2 1_455 5_656 180.0(5)
O2 Gd1 O2 1_455 7_546 111.68(7)
O2 Gd1 O2 1_455 7_556 111.68(7)
O2 Gd1 O3 1_455 1_445 55.84(5)
O2 Gd1 O3 1_455 1_455 55.84(5)
O2 Gd1 O3 1_455 1_545 124.16(5)
O2 Gd1 O3 1_455 . 124.16(5)
O2 Gd1 O2 . 3_545 68.32(7)
O2 Gd1 O2 . 3_555 68.32(7)
O2 Gd1 O2 . 5_556 180.0(5)
O2 Gd1 O2 . 5_656 74.86(13)
O2 Gd1 O2 . 7_546 111.68(7)
O2 Gd1 O2 . 7_556 111.68(7)
O2 Gd1 O3 . 1_445 124.16(5)
O2 Gd1 O3 . 1_455 124.16(5)
O2 Gd1 O3 . 1_545 55.84(5)
O2 Gd1 O3 . . 55.84(5)
O2 Gd1 O2 3_545 3_555 105.14(13)
O2 Gd1 O2 3_545 5_556 111.68(7)
O2 Gd1 O2 3_545 5_656 111.68(7)
O2 Gd1 O2 3_545 7_546 74.86(13)
O2 Gd1 O2 3_545 7_556 180.0(5)
O2 Gd1 O3 3_545 1_445 55.84(5)
O2 Gd1 O3 3_545 1_455 124.16(5)
O2 Gd1 O3 3_545 1_545 55.84(5)
O2 Gd1 O3 3_545 . 124.16(5)
O2 Gd1 O2 3_555 5_556 111.68(7)
O2 Gd1 O2 3_555 5_656 111.68(7)
O2 Gd1 O2 3_555 7_546 180.0(5)
O2 Gd1 O2 3_555 7_556 74.86(13)
O2 Gd1 O3 3_555 1_445 124.16(5)
O2 Gd1 O3 3_555 1_455 55.84(5)
O2 Gd1 O3 3_555 1_545 124.16(5)
O2 Gd1 O3 3_555 . 55.84(5)
O2 Gd1 O2 5_556 5_656 105.14(13)
O2 Gd1 O2 5_556 7_546 68.32(7)
O2 Gd1 O2 5_556 7_556 68.32(7)
O2 Gd1 O3 5_556 1_445 55.84(5)
O2 Gd1 O3 5_556 1_455 55.84(5)
O2 Gd1 O3 5_556 1_545 124.16(5)
O2 Gd1 O3 5_556 . 124.16(5)
O2 Gd1 O2 5_656 7_546 68.32(7)
O2 Gd1 O2 5_656 7_556 68.32(7)
O2 Gd1 O3 5_656 1_445 124.16(5)
O2 Gd1 O3 5_656 1_455 124.16(5)
O2 Gd1 O3 5_656 1_545 55.84(5)
O2 Gd1 O3 5_656 . 55.84(5)
O2 Gd1 O2 7_546 7_556 105.14(13)
O2 Gd1 O3 7_546 1_445 55.84(5)
O2 Gd1 O3 7_546 1_455 124.16(5)
O2 Gd1 O3 7_546 1_545 55.84(5)
O2 Gd1 O3 7_546 . 124.16(5)
O2 Gd1 O3 7_556 1_445 124.16(5)
O2 Gd1 O3 7_556 1_455 55.84(5)
O2 Gd1 O3 7_556 1_545 124.16(5)
O2 Gd1 O3 7_556 . 55.84(5)
O3 Gd1 O3 1_445 1_455 90.000(8)
O3 Gd1 O3 1_445 1_545 90.000(8)
O3 Gd1 O3 1_445 . 180.0(5)
O3 Gd1 O3 1_455 1_545 180.0(5)
O3 Gd1 O3 1_455 . 90.000(8)
O3 Gd1 O3 1_545 . 90.000(8)
O1 Ba1 O1 1_445 1_455 90.000(8)
O1 Ba1 O1 1_445 1_545 90.000(8)
O1 Ba1 O1 1_445 . 180.0(5)
O1 Ba1 O2 1_445 1_455 62.68(4)
O1 Ba1 O2 1_445 . 117.32(4)
O1 Ba1 O2 1_445 3_545 62.68(4)
O1 Ba1 O2 1_445 3_555 117.32(4)
O1 Ba1 O2 1_445 5_555 62.68(4)
O1 Ba1 O2 1_445 5_655 117.32(4)
O1 Ba1 O2 1_445 7_545 62.68(4)
O1 Ba1 O2 1_445 7_555 117.32(4)
O1 Ba1 O1 1_455 1_545 180.0(5)
O1 Ba1 O1 1_455 . 90.000(8)
O1 Ba1 O2 1_455 1_455 62.68(4)
O1 Ba1 O2 1_455 . 117.32(4)
O1 Ba1 O2 1_455 3_545 117.32(4)
O1 Ba1 O2 1_455 3_555 62.68(4)
O1 Ba1 O2 1_455 5_555 62.68(4)
O1 Ba1 O2 1_455 5_655 117.32(4)
O1 Ba1 O2 1_455 7_545 117.32(4)
O1 Ba1 O2 1_455 7_555 62.68(4)
O1 Ba1 O1 1_545 . 90.000(8)
O1 Ba1 O2 1_545 1_455 117.32(4)
O1 Ba1 O2 1_545 . 62.68(4)
O1 Ba1 O2 1_545 3_545 62.68(4)
O1 Ba1 O2 1_545 3_555 117.32(4)
O1 Ba1 O2 1_545 5_555 117.32(4)
O1 Ba1 O2 1_545 5_655 62.68(4)
O1 Ba1 O2 1_545 7_545 62.68(4)
O1 Ba1 O2 1_545 7_555 117.32(4)
O1 Ba1 O2 . 1_455 117.32(4)
O1 Ba1 O2 . . 62.68(4)
O1 Ba1 O2 . 3_545 117.32(4)
O1 Ba1 O2 . 3_555 62.68(4)
O1 Ba1 O2 . 5_555 117.32(4)
O1 Ba1 O2 . 5_655 62.68(4)
O1 Ba1 O2 . 7_545 117.32(4)
O1 Ba1 O2 . 7_555 62.68(4)
O2 Ba1 O2 1_455 . 80.94(9)
O2 Ba1 O2 1_455 3_545 54.64(5)
O2 Ba1 O2 1_455 3_555 54.64(5)
O2 Ba1 O2 1_455 5_555 99.06(9)
O2 Ba1 O2 1_455 5_655 180.0(5)
O2 Ba1 O2 1_455 7_545 125.36(5)
O2 Ba1 O2 1_455 7_555 125.36(5)
O2 Ba1 O2 . 3_545 54.64(5)
O2 Ba1 O2 . 3_555 54.64(5)
O2 Ba1 O2 . 5_555 180.0(5)
O2 Ba1 O2 . 5_655 99.06(9)
O2 Ba1 O2 . 7_545 125.36(5)
O2 Ba1 O2 . 7_555 125.36(5)
O2 Ba1 O2 3_545 3_555 80.94(9)
O2 Ba1 O2 3_545 5_555 125.36(5)
O2 Ba1 O2 3_545 5_655 125.36(5)
O2 Ba1 O2 3_545 7_545 99.06(9)
O2 Ba1 O2 3_545 7_555 180.0(5)
O2 Ba1 O2 3_555 5_555 125.36(5)
O2 Ba1 O2 3_555 5_655 125.36(5)
O2 Ba1 O2 3_555 7_545 180.0(5)
O2 Ba1 O2 3_555 7_555 99.06(9)
O2 Ba1 O2 5_555 5_655 80.94(9)
O2 Ba1 O2 5_555 7_545 54.64(5)
O2 Ba1 O2 5_555 7_555 54.64(5)
O2 Ba1 O2 5_655 7_545 54.64(5)
O2 Ba1 O2 5_655 7_555 54.64(5)
O2 Ba1 O2 7_545 7_555 80.94(9)
O1 Co1 O2 . . 100.51(14)
O1 Co1 O2 . 1_565 100.51(14)
O1 Co1 O2 . 3_555 100.51(14)
O1 Co1 O2 . 3_655 100.51(14)
O1 Co1 O3 . . 180.0(5)
O2 Co1 O2 . 1_565 159.0(2)
O2 Co1 O2 . 3_555 88.09(4)
O2 Co1 O2 . 3_655 88.09(4)
O2 Co1 O3 . . 79.49(14)
O2 Co1 O2 1_565 3_555 88.09(4)
O2 Co1 O2 1_565 3_655 88.09(4)
O2 Co1 O3 1_565 . 79.49(14)
O2 Co1 O2 3_555 3_655 159.0(2)
O2 Co1 O3 3_555 . 79.49(14)
O2 Co1 O3 3_655 . 79.49(14)
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
Gd1 O2 1_455 2.455(3)
Gd1 O2 . 2.455(3)
Gd1 O2 3_545 2.455(3)
Gd1 O2 3_555 2.455(3)
Gd1 O2 5_556 2.455(3)
Gd1 O2 5_656 2.455(3)
Gd1 O2 7_546 2.455(3)
Gd1 O2 7_556 2.455(3)
Gd1 O3 1_445 2.7566(4)
Gd1 O3 1_455 2.7566(4)
Gd1 O3 1_545 2.7566(4)
Gd1 O3 . 2.7566(4)
Ba1 O1 1_445 2.7566(4)
Ba1 O1 1_455 2.7566(4)
Ba1 O1 1_545 2.7566(4)
Ba1 O1 . 2.7566(4)
Ba1 O2 1_455 3.003(4)
Ba1 O2 . 3.003(4)
Ba1 O2 3_545 3.003(4)
Ba1 O2 3_555 3.003(4)
Ba1 O2 5_555 3.003(4)
Ba1 O2 5_655 3.003(4)
Ba1 O2 7_545 3.003(4)
Ba1 O2 7_555 3.003(4)
Co1 O1 . 1.9230(11)
Co1 O2 . 1.9825(10)
Co1 O2 1_565 1.9825(10)
Co1 O2 3_555 1.9825(10)
Co1 O2 3_655 1.9825(10)
Co1 O3 . 1.8536(11)
